# Microwave-assisted solution synthesis of metastable intergrowth of AgInS2 polymorphs

Adedoyin Adeyemi, Rae Ann Earnest, Tori Cox, Oleg Lebedev, Julia Zaikina

► To cite this version:

Adedoyin Adeyemi, Rae Ann Earnest, Tori Cox, Oleg Lebedev, Julia Zaikina. Microwave-assisted solution synthesis of metastable intergrowth of AgInS2 polymorphs. Molecules, 2022, 27 (6), pp.1815. 10.3390/molecules27061815. [https://doi.org/10.3390/molecules27061815](https://doi.org/10.3390/molecules27061815)

HAL Id: hal-03817358

https://hal.science/hal-03817358

Submitted on 24 May 2024

HAL is a multi-disciplinary open access
archive for the deposit and dissemination of sci-
entific research documents, whether they are pub-
lished or not. The documents may come from
teaching and research institutions in France or
abroad, or from public or private research centers.

L'archive ouverte pluridisciplinaire HAL, est
destinée au dépôt et à la diffusion de documents
scientifiques de niveau recherche, publiés ou non,
émanant des établissements d'enseignement et de
recherche français ou étrangers, des laboratoires
publics ou privés.

<figure><img src="image_1.png" /></figure>

Distributed under a Creative Commons Attribution 4.0 International License
Article

# Microwave-Assisted Solution Synthesis of Metastable Intergrowth of AgInS₂ Polymorphs

Adedoyin N. Adeyemi<fnref n="1" />, Rae Ann Earnest<fnref n="1" />, Tori Cox<fnref n="1" />, Oleg I. Lebedev<fnref n="2" /> and Julia V. Zaikina <fnref n="1" />,*

**Abstract:** The intergrowth of stable and metastable AgInS₂ polymorphs was synthesized using a microwave-assisted synthesis. The samples were synthesized in water and in a deep eutectic solvent (DES) consisting of choline chloride and thiourea. An increase in the metal precursor concentration improved the crystallinity of the synthesized samples and affected the particle size. AgInS₂ cannot be synthesized from crystalline binary Ag₂S or In₂S₃ via this route. The solution synthesis reported here results in the intergrowth of the thermodynamically stable polymorph (space group *I*42d, chalcopyrite structure) and the high-temperature polymorph (space group *P*na21, wurtzite-like structure) that is metastable at room temperature. A scanning transmission microscopy (STEM) study revealed the intergrowth of tetragonal and orthorhombic polymorphs in a single particle and unambiguously established that the long-thought hexagonal wurtzite polymorph has pseudo-hexagonal symmetry and is best described with the orthorhombic unit cell. The solution-synthesized AgInS₂ polymorphs intergrowth has slightly lower bandgap values in the range of 1.73 eV–1.91 eV compared to the previously reported values for tetragonal *I*42d (1.86 eV) and orthorhombic *P*na21 (1.98 eV) polymorphs.

**Keywords:** metastable; deep eutectic solvent (DES); morphology; STEM; semiconductor; green synthesis

## 1. Introduction

Deep eutectic solvents (DESs) are emerging solvents that are analogs of ionic liquids [1]. DESs are made by mixing a hydrogen bond donor and a hydrogen bond acceptor (usually a quaternary ammonium salt) in a specific molar ratio [1,2]. The eutectic mixture of the two DES constituents has a significantly lower melting point compared to its individual components because of the hydrogen bonding occurring in the mixture; hence a viscous liquid is formed [1,3]. DESs have high solubility rates for metal precursors, such as salts and binary oxides [4]; therefore, DESs have been used as the reaction medium in the synthesis of functional oxides [5–8], including a metastable oxide [9]. Due to the various possible combinations of hydrogen bond donors and acceptors, DESs allow for synthetic tunability and have also been employed in the syntheses of sulfides [10–12].

AgInS₂ is one of the two ternary sulfides reported in the pseudo-binary Ag₂S-In₂S₃ system. AgInS₂ is reported to have four polymorphic modifications. The most common room-temperature polymorph has a tetragonal chalcopyrite structure (space group *I*42d) [13], which transforms into the high-temperature orthorhombic wurtzite-like structure (space group *P*na21) [14] upon heating to ~620 °C [15]. The less common polymorphs are the hexagonal (space group *P*6₃mc) [13] wurtzite structure and the trigonal structure (space group *R*3m), the latter one was synthesized under high-pressure and high-temperature conditions [16]. The structures of the *I*42d, *P*na21, and *P*6₃mc polymorphs comprise of the Ag- and In- centered AgS₄ and InS₄ tetrahedra that share corners to give different types of

<figure><img src="image_1.png" /></figure>

check for
updates

**Citation:** Adeyemi, A.N.; Earnest, R.A.; Cox, T.; Lebedev, O.I.; Zaikina, J.V. Microwave-Assisted Solution Synthesis of Metastable Intergrowth of AgInS₂ Polymorphs. *Molecules* **2022**, *27*, 1815. https://doi.org/10.3390/molecules27061815

Academic Editor: Paul A. Maggard

Received: 1 February 2022

Accepted: 1 March 2022

Published: 10 March 2022

**Publisher's Note:** MDPI stays neutral with regard to jurisdictional claims in published maps and institutional affiliations.

<figure><img src="image_2.png" /></figure>

**Copyright:** © 2022 by the authors. Licensee MDPI, Basel, Switzerland. This article is an open access article distributed under the terms and conditions of the Creative Commons Attribution (CC BY) license (https://creativecommons.org/licenses/by/4.0/).

<footnote n="1">¹ Department of Chemistry, Iowa State University, Ames, IA 50011, USA; nifemi@iastate.edu (A.N.A.); rearnest@iastate.edu (R.A.E.); tlcox@iastate.edu (T.C.)</footnote>

<footnote n="2">² Laboratoire Crismat, ENSICAEN, CNRS UMR 6508, 14050 Caen, France; oleg.lebedev@ensicaen.fr</footnote>

<footnote>* Correspondence: yzaikina@iastate.edu</footnote>
Article

# Microwave-Assisted Solution Synthesis of Metastable Intergrowth of AgInS₂ Polymorphs

Adedoyin N. Adeyemi<fnref n="1" />, Rae Ann Earnest<fnref n="1" />, Tori Cox<fnref n="1" />, Oleg I. Lebedev<fnref n="2" /> and Julia V. Zaikina <fnref n="1" />,*

**Abstract:** The intergrowth of stable and metastable AgInS₂ polymorphs was synthesized using a microwave-assisted synthesis. The samples were synthesized in water and in a deep eutectic solvent (DES) consisting of choline chloride and thiourea. An increase in the metal precursor concentration improved the crystallinity of the synthesized samples and affected the particle size. AgInS₂ cannot be synthesized from crystalline binary Ag₂S or In₂S₃ via this route. The solution synthesis reported here results in the intergrowth of the thermodynamically stable polymorph (space group *I*42d, chalcopyrite structure) and the high-temperature polymorph (space group *P*na21, wurtzite-like structure) that is metastable at room temperature. A scanning transmission microscopy (STEM) study revealed the intergrowth of tetragonal and orthorhombic polymorphs in a single particle and unambiguously established that the long-thought hexagonal wurtzite polymorph has pseudo-hexagonal symmetry and is best described with the orthorhombic unit cell. The solution-synthesized AgInS₂ polymorphs intergrowth has slightly lower bandgap values in the range of 1.73 eV–1.91 eV compared to the previously reported values for tetragonal *I*42d (1.86 eV) and orthorhombic *P*na21 (1.98 eV) polymorphs.

**Keywords:** metastable; deep eutectic solvent (DES); morphology; STEM; semiconductor; green synthesis

## 1. Introduction

Deep eutectic solvents (DESs) are emerging solvents that are analogs of ionic liquids [1]. DESs are made by mixing a hydrogen bond donor and a hydrogen bond acceptor (usually a quaternary ammonium salt) in a specific molar ratio [1,2]. The eutectic mixture of the two DES constituents has a significantly lower melting point compared to its individual components because of the hydrogen bonding occurring in the mixture; hence a viscous liquid is formed [1,3]. DESs have high solubility rates for metal precursors, such as salts and binary oxides [4]; therefore, DESs have been used as the reaction medium in the synthesis of functional oxides [5–8], including a metastable oxide [9]. Due to the various possible combinations of hydrogen bond donors and acceptors, DESs allow for synthetic tunability and have also been employed in the syntheses of sulfides [10–12].

AgInS₂ is one of the two ternary sulfides reported in the pseudo-binary Ag₂S-In₂S₃ system. AgInS₂ is reported to have four polymorphic modifications. The most common room-temperature polymorph has a tetragonal chalcopyrite structure (space group *I*42d) [13], which transforms into the high-temperature orthorhombic wurtzite-like structure (space group *P*na21) [14] upon heating to ~620 °C [15]. The less common polymorphs are the hexagonal (space group *P*6₃mc) [13] wurtzite structure and the trigonal structure (space group *R*3m), the latter one was synthesized under high-pressure and high-temperature conditions [16]. The structures of the *I*42d, *P*na21, and *P*6₃mc polymorphs comprise of the Ag- and In- centered AgS₄ and InS₄ tetrahedra that share corners to give different types of

<figure><img src="image_2.png" /></figure>

check for
updates

**Citation:** Adeyemi, A.N.; Earnest, R.A.; Cox, T.; Lebedev, O.I.; Zaikina, J.V. Microwave-Assisted Solution Synthesis of Metastable Intergrowth of AgInS₂ Polymorphs. *Molecules* **2022**, *27*, 1815. https://doi.org/10.3390/molecules27061815

Academic Editor: Paul A. Maggard

Received: 1 February 2022

Accepted: 1 March 2022

Published: 10 March 2022

**Publisher's Note:** MDPI stays neutral with regard to jurisdictional claims in published maps and institutional affiliations.

<figure><img src="image_3.png" /></figure>

**Copyright:** © 2022 by the authors. Licensee MDPI, Basel, Switzerland. This article is an open access article distributed under the terms and conditions of the Creative Commons Attribution (CC BY) license (https://creativecommons.org/licenses/by/4.0/).

<footnote n="1">¹ Department of Chemistry, Iowa State University, Ames, IA 50011, USA; nifemi@iastate.edu (A.N.A.); rearnest@iastate.edu (R.A.E.); tlcox@iastate.edu (T.C.)</footnote>

<footnote n="2">² Laboratoire Crismat, ENSICAEN, CNRS UMR 6508, 14050 Caen, France; oleg.lebedev@ensicaen.fr</footnote>

<footnote>* Correspondence: yzaikina@iastate.edu</footnote>
packing (Figure 1). The I̅42d polymorph is made of double layers of AgS₄ tetrahedra alternating with double layers of InS₄ tetrahedra. The I̅42d chalcopyrite structure is an ordered variant of a cubic sphalerite. The *Pna2*₁ polymorph has a wurtzite structure, where Ag and In cations share the same crystallographic site. The high-temperature *Pna2*₁ polymorph has a pseudo-wurtzite structure, where Ag and In are ordered in different crystallographic sites, resulting in the similar alternating layers of InS₄ and AgS₄ tetrahedra as in the wurtzite structure, but with the lowering of the symmetry to orthorhombic. The unit cell parameters of the *Pna2*₁ and the *P6₃mc* structures are related as follows: *a*<sub>ortho</sub> = √3*a*<sub>hex</sub>, *b*<sub>ortho</sub> = 2*a*<sub>hex</sub>, and *c*<sub>ortho</sub> ~ *c*<sub>hex</sub>; where *ortho* represents *Pna2*₁ and *hex* represents *P6₃mc* [17].

<figure><img src="image_3.png" /><figcaption>**Figure 1.** The crystal structures of the tetragonal, orthorhombic, and hexagonal polymorphs of AgInS₂. Atoms are color-coded: In—purple, Ag—gray, S—yellow, and the site with mixed In/Ag occupancy is denoted as a half-purple and half-grey sphere. The unit cell is shown with a black line. The orientation is chosen to highlight similarities in the structures of polymorphs.</figcaption></figure>

According to the Materials Project Database [18], the I̅42d polymorph is thermodynamically stable, the high-temperature *Pna2*₁ polymorph is metastable by ~0.008 eV/atom, and the high-pressure *R*3*m* structure is metastable by 0.090 eV/atom. No information was found for the *P6*₃*m* polymorph in the Materials Project Database; however, a trigonal *P*3*m*1 structure with similar unit cell parameters as the *P6*₃*m* polymorph and ordered arrangement of Ag and In cations is calculated to be metastable by ~0.97 eV/atom. A closer inspection of the publication reporting synthesis of wurtzite polymorph reveals that the structure assignment was done based on powder X-ray diffraction data collected for a multiphase sample that also contained a tetragonal polymorph [13]. Thus, the question regarding the validity of these data arises.

AgInS₂ are currently being explored as non-toxic alternatives for photoluminescent compounds, such as the commercialized CdSe, because the size-dependent bandgap of AgInS₂ falls within the visible light region [19–21]. However, the broad photoluminescent spectra, which is a result of the lack of monochromaticity, is a major challenge [22,23].

Here, we studied the microwave-assisted solution synthesis of AgInS₂ using two solvents—DI water and a DES consisting of choline chloride and thiourea. We investigated the effect of the heating profile, solvents (DI water vs. DES), and metal precursor concentration on the synthesis of the AgInS₂ polymorphs. The synthetic route resulted in the intergrowth of two polymorphs of AgInS₂: the I̅42d and high-temperature *Pna2*₁ structures. We also investigated the thermal stability of the metastable intergrowth of two AgInS₂ polymorphs using in-situ high-temperature powder X-ray diffraction. We further used scanning transmission electron microscopy to address a controversy regarding the hexagonal *P6*₃*m* polymorph with a wurtzite structure.
packing (Figure 1). The I̅42d polymorph is made of double layers of AgS₄ tetrahedra alternating with double layers of InS₄ tetrahedra. The I̅42d chalcopyrite structure is an ordered variant of a cubic sphalerite. The *Pna2*₁ polymorph has a wurtzite structure, where Ag and In cations share the same crystallographic site. The high-temperature *Pna2*₁ polymorph has a pseudo-wurtzite structure, where Ag and In are ordered in different crystallographic sites, resulting in the similar alternating layers of InS₄ and AgS₄ tetrahedra as in the wurtzite structure, but with the lowering of the symmetry to orthorhombic. The unit cell parameters of the *Pna2*₁ and the *P6₃mc* structures are related as follows: *a*<sub>ortho</sub> = √3*a*<sub>hex</sub>, *b*<sub>ortho</sub> = 2*a*<sub>hex</sub>, and *c*<sub>ortho</sub> ~ *c*<sub>hex</sub>; where *ortho* represents *Pna2*₁ and *hex* represents *P6₃mc* [17].

<figure><img src="image_4.png" /><figcaption>**Figure 1.** The crystal structures of the tetragonal, orthorhombic, and hexagonal polymorphs of AgInS₂. Atoms are color-coded: In—purple, Ag—gray, S—yellow, and the site with mixed In/Ag occupancy is denoted as a half-purple and half-grey sphere. The unit cell is shown with a black line. The orientation is chosen to highlight similarities in the structures of polymorphs.</figcaption></figure>

According to the Materials Project Database [18], the I̅42d polymorph is thermodynamically stable, the high-temperature *Pna2*₁ polymorph is metastable by ~0.008 eV/atom, and the high-pressure *R*₃*m* structure is metastable by 0.090 eV/atom. No information was found for the *P6₃mc* wurtzite polymorph in the Materials Project Database; however, a trigonal *P*3*m*1 structure with similar unit cell parameters as the *P6₃mc* polymorph and ordered arrangement of Ag and In cations is calculated to be metastable by ~0.97 eV/atom. A closer inspection of the publication reporting synthesis of wurtzite polymorph reveals that the structure assignment was done based on powder X-ray diffraction data collected for a multiphase sample that also contained a tetragonal polymorph [13]. Thus, the question regarding the validity of these data arises.

AgInS₂ are currently being explored as non-toxic alternatives for photoluminescent compounds, such as the commercialized CdSe, because the size-dependent bandgap of AgInS₂ falls within the visible light region [19–21]. However, the broad photoluminescent spectra, which is a result of the lack of monochromaticity, is a major challenge [22,23].

Here, we studied the microwave-assisted solution synthesis of AgInS₂ using two solvents—DI water and a DES consisting of choline chloride and thiourea. We investigated the effect of the heating profile, solvents (DI water vs. DES), and metal precursor concentration on the synthesis of the AgInS₂ polymorphs. The synthetic route resulted in the intergrowth of two polymorphs of AgInS₂: the I̅42d and high-temperature *Pna2*₁ structures. We also investigated the thermal stability of the metastable intergrowth of two AgInS₂ polymorphs using in-situ high-temperature powder X-ray diffraction. We further used scanning transmission electron microscopy to address a controversy regarding the hexagonal *P6₃mc* polymorph with a wurtzite structure.
## 2. Results and Discussion

A deep eutectic solvent utilized in this work consists of choline chloride as a hydrogen bond acceptor (melting point of 302 °C) and thiourea as both the hydrogen bond donor and the sulfur source (melting point of 182 °C). The eutectic mixture of choline chloride and thiourea in a 1:2 molar ratio exhibits a lower melting point of 69 °C compared to its components [2]. AgNO₃ and InCl₃·xH₂O are utilized as the metal precursors in this work since they have appreciable solubility in the chosen DES [2]. The DES-assisted synthesis utilized in this work is similar to a previously reported solvothermal synthesis of binary sulfide using a DES consisting of choline chloride and thioacetamide, where thioacetamide is the hydrogen bond donor and also a sulfur source [11].

For the microwave solution synthesis of AgInS₂, we studied two temperature profiles: 1-step and 2-step heating profiles (see Experimental for details). For both profiles, the highest synthesis temperature was set to 180 °C above which thiourea will decompose, while the 2-step profile included additional heating at 80 °C to ensure the dissolution of the metal precursors before ramping to 180 °C. We compared the syntheses utilizing DES, or deionized water, as a solvent. Furthermore, we varied concentrations of the metal precursors and observed that the variation in the amount of the metal precursors affected the crystallinity, particle size, and shape. Separately, we studied the reaction mechanism for the synthesis of AgInS₂ and ruled out a partial cation exchange between a crystalline binary sulfide (Ag₂S or In₂S₃) and a cation in the solution (In⁺³ and Ag⁺, respectively) as a possible mechanism. The reaction between the crystalline pre-synthesized Ag₂S with the aqueous solution of InCl₃·H₂O did not proceed, while the metathesis reaction of the crystalline pre-synthesized In₂S₃ with an aqueous solution of AgNO₃ resulted in the formation of Ag₂S. Further details of this study can be found in the Supplementary Materials.

1-step synthesis. Samples of AgInS₂ synthesized using the 1-step synthesis contained two polymorphs, regardless of the used solvent: the high-temperature orthorhombic *Pna*2₁ and the tetragonal *I*42*d* polymorphs. Varying molar concentrations of the metal precursors in the solution were employed in both the water and DES. However, we observed very similar powder X-ray diffraction (PXRD) patterns in all the 1-step syntheses, as shown in Figure 2. This suggests that the two polymorphs are present in similar ratios in all the 1-step-synthesized samples, irrespective of the solvent or metal precursor concentration employed. The dominant polymorph is the tetragonal *I*42*d* polymorph.

The crystallinity of the phases was qualitatively evaluated by tracking the full width at half maximum (FWHM) of the most intense diffraction peak at ~26.6°. Narrower peaks indicate a higher crystallinity. According to the PXRD data, the peaks of the orthorhombic *Pna*2₁ polymorph are better resolved in the samples made with water than in the samples made in the DES, indicating improved crystallinity. Comparing the FWHM of the 0.5 mmol sample made in the DES (0.273) and that made in water (0.235), we see that the sample made in water has a slightly better crystallinity. The crystallinity of the synthesized samples also increases with an increase in the metal precursor concentration in both water and DES. This is more significant for the DES-made samples, as seen in Figure 2, where the 3 mmol sample (FWHM of 0.231) is more crystalline than the 0.5 mmol sample (FWHM of 0.273).

The morphology and particle size were also analyzed by scanning electron microscopy (SEM). As seen in the SEM images (Figure 3), the 1-step water-synthesized AgInS₂ have plate-like morphologies arranged like flower petals, and the morphology is uniform throughout the sample. The uniform morphology may also suggest a metastable inter-growth of the orthorhombic *Pna*2₁ and the tetragonal *I*42*d* polymorphs in a single particle. Notably, an increase in the metal precursor concentration of the 1-step water-synthesized AgInS₂ leads to an increase in the particle size. The particle size in the 0.1 mmol sample is evidently smaller than in the 0.5 mmol sample. Further increase in concentration to 1 mmol leads to even larger particles, consistent with the PXRD data. The samples with larger particle sizes (0.5 and 1 mmol 1-step water-synthesized AgInS₂) have peaks in PXRD patterns that are more narrow and better-resolved than the samples with the smaller particle size
## 2. Results and Discussion

A deep eutectic solvent utilized in this work consists of choline chloride as a hydrogen bond acceptor (melting point of 302 °C) and thiourea as both the hydrogen bond donor and the sulfur source (melting point of 182 °C). The eutectic mixture of choline chloride and thiourea in a 1:2 molar ratio exhibits a lower melting point of 69 °C compared to its components [2]. AgNO₃ and InCl₃·xH₂O are utilized as the metal precursors in this work since they have appreciable solubility in the chosen DES [2]. The DES-assisted synthesis utilized in this work is similar to a previously reported solvothermal synthesis of binary sulfide using a DES consisting of choline chloride and thioacetamide, where thioacetamide is the hydrogen bond donor and also a sulfur source [11].

For the microwave solution synthesis of AgInS₂, we studied two temperature profiles: 1-step and 2-step heating profiles (see Experimental for details). For both profiles, the highest synthesis temperature was set to 180 °C above which thiourea will decompose, while the 2-step profile included additional heating at 80 °C to ensure the dissolution of the metal precursors before ramping to 180 °C. We compared the syntheses utilizing DES, or deionized water, as a solvent. Furthermore, we varied concentrations of the metal precursors and observed that the variation in the amount of the metal precursors affected the crystallinity, particle size, and shape. Separately, we studied the reaction mechanism for the synthesis of AgInS₂ and ruled out a partial cation exchange between a crystalline binary sulfide (Ag₂S or In₂S₃) and a cation in the solution (In⁺³ and Ag⁺, respectively) as a possible mechanism. The reaction between the crystalline pre-synthesized Ag₂S with the aqueous solution of InCl₃·H₂O did not proceed, while the metathesis reaction of the crystalline pre-synthesized In₂S₃ with an aqueous solution of AgNO₃ resulted in the formation of Ag₂S. Further details of this study can be found in the Supplementary Materials.

1-step synthesis. Samples of AgInS₂ synthesized using the 1-step synthesis contained two polymorphs, regardless of the used solvent: the high-temperature orthorhombic *Pna*2₁ and the tetragonal *I*42*d* polymorphs. Varying molar concentrations of the metal precursors in the solution were employed in both the water and DES. However, we observed very similar powder X-ray diffraction (PXRD) patterns in all the 1-step syntheses, as shown in Figure 2. This suggests that the two polymorphs are present in similar ratios in all the 1-step-synthesized samples, irrespective of the solvent or metal precursor concentration employed. The dominant polymorph is the tetragonal *I*42*d* polymorph.

The crystallinity of the phases was qualitatively evaluated by tracking the full width at half maximum (FWHM) of the most intense diffraction peak at ~26.6°. Narrower peaks indicate a higher crystallinity. According to the PXRD data, the peaks of the orthorhombic *Pna*2₁ polymorph are better resolved in the samples made with water than in the samples made in the DES, indicating improved crystallinity. Comparing the FWHM of the 0.5 mmol sample made in the DES (0.273) and that made in water (0.235), we see that the sample made in water has a slightly better crystallinity. The crystallinity of the synthesized samples also increases with an increase in the metal precursor concentration in both water and DES. This is more significant for the DES-made samples, as seen in Figure 2, where the 3 mmol sample (FWHM of 0.231) is more crystalline than the 0.5 mmol sample (FWHM of 0.273).

The morphology and particle size were also analyzed by scanning electron microscopy (SEM). As seen in the SEM images (Figure 3), the 1-step water-synthesized AgInS₂ have plate-like morphologies arranged like flower petals, and the morphology is uniform throughout the sample. The uniform morphology may also suggest a metastable inter-growth of the orthorhombic *Pna*2₁ and the tetragonal *I*42*d* polymorphs in a single particle. Notably, an increase in the metal precursor concentration of the 1-step water-synthesized AgInS₂ leads to an increase in the particle size. The particle size in the 0.1 mmol sample is evidently smaller than in the 0.5 mmol sample. Further increase in concentration to 1 mmol leads to even larger particles, consistent with the PXRD data. The samples with larger particle sizes (0.5 and 1 mmol 1-step water-synthesized AgInS₂) have peaks in PXRD patterns that are more narrow and better-resolved than the samples with the smaller particle size
synthesized from the less-concentrated solution (0.1 mmol 1-step water-synthesized AgInS₂).

<figure><img src="image_4.png" /><figcaption>**Figure 2.** PXRD patterns of the 1-step synthesis of water (blue shaded region) and DES-synthesized (orange shaded region) AgInS₂ with varying concentrations of metal precursors. Diffraction peaks for Ag₂S impurity are denoted with an asterisk (*). The theoretical PXRD patterns include ICSD 51617, representing the *I*̅42*d; ICSD 76276, representing the *P*6₃mc; and ICSD 605408, representing the *P*na2₁ polymorph.</figcaption></figure>

The SEM images of the *1-step* DES-synthesized AgInS₂ show that the particles also have plate-like morphologies, with varying arrangements depending on the metal precursor concentration. The most dilute concentration in the *1-step* DES-synthesized AgInS₂ (0.5 mmol sample) shows a flower, petal-like arrangement (Figure 3d), which is identical to the arrangement exhibited by the *1-step* water-synthesized AgInS₂. As we increased the metal precursor concentration to 1 mmol, the plate-like particles of the *1-step* DES-synthesized AgInS₂ exhibited an arrangement of small, stacked plates, as shown in Figure 3e. Increasing the metal precursor concentration further to 3 mmol led to larger stacked plates, as shown in Figure 3f.

*2-step* synthesis. We further explored a *2-step* synthesis of AgInS₂, where reagents were dwelled at 80 °C to allow for the proper mixing and complete dissolution of the precursors before ramping to 180 °C. We discovered that the effect of the solvent used and the metal precursor concentration was more significant in the *2-step* synthesis of AgInS₂. We observed changes in the amount of impurities present and the ratios between the polymorphs in the *2-step*-synthesized samples as we varied the solvent and the metal precursor concentration (Figure 4). From the distinct PXRD pattern, we suspect that the *2-step*-synthesized AgInS₂ at a dilute metal precursor concentration of 0.1 mmol for water and 0.5 mmol for DES syntheses are a mixture of the hexagonal *P*6₃mc polymorph and the tetragonal *I*̅42*d polymorph. However, given that the observed peaks are broad, indicating a low crystallinity of the sample, and that the PXRD patterns of the wurtzite *P*6₃mc and *P*na2₁ polymorphs are similar, the formation of wurtzite *P*6₃mc polymorph, based on PXRD data only, cannot be ascertained. The further increase of the metal precursor concentration led to a mixture of the orthorhombic *P*na2₁ and the tetragonal *I*̅42*d polymorphs, similar to
synthesized from the less-concentrated solution (0.1 mmol 1-step water-synthesized AgInS₂).

<figure><img src="image_5.png" /><figcaption>**Figure 2.** PXRD patterns of the 1-step synthesis of water (blue shaded region) and DES-synthesized (orange shaded region) AgInS₂ with varying concentrations of metal precursors. Diffraction peaks for Ag₂S impurity are denoted with an asterisk (*). The theoretical PXRD patterns include ICSD 51617, representing the *I*̅42*d; ICSD 76276, representing the *P*6₃mc; and ICSD 605408, representing the *P*na2₁ polymorph.</figcaption></figure>

The SEM images of the *1-step* DES-synthesized AgInS₂ show that the particles also have plate-like morphologies, with varying arrangements depending on the metal precursor concentration. The most dilute concentration in the *1-step* DES-synthesized AgInS₂ (0.5 mmol sample) shows a flower, petal-like arrangement (Figure 3d), which is identical to the arrangement exhibited by the *1-step* water-synthesized AgInS₂. As we increased the metal precursor concentration to 1 mmol, the plate-like particles of the *1-step* DES-synthesized AgInS₂ exhibited an arrangement of small, stacked plates, as shown in Figure 3e. Increasing the metal precursor concentration further to 3 mmol led to larger stacked plates, as shown in Figure 3f.

*2-step* synthesis. We further explored a *2-step* synthesis of AgInS₂, where reagents were dwelled at 80 °C to allow for the proper mixing and complete dissolution of the precursors before ramping to 180 °C. We discovered that the effect of the solvent used and the metal precursor concentration was more significant in the *2-step* synthesis of AgInS₂. We observed changes in the amount of impurities present and the ratios between the polymorphs in the *2-step*-synthesized samples as we varied the solvent and the metal precursor concentration (Figure 4). From the distinct PXRD pattern, we suspect that the *2-step*-synthesized AgInS₂ at a dilute metal precursor concentration of 0.1 mmol for water and 0.5 mmol for DES syntheses are a mixture of the hexagonal *P*6₃mc polymorph and the tetragonal *I*̅42*d polymorph. However, given that the observed peaks are broad, indicating a low crystallinity of the sample, and that the PXRD patterns of the wurtzite *P*6₃mc and *P*na2₁ polymorphs are similar, the formation of wurtzite *P*6₃mc polymorph, based on PXRD data only, cannot be ascertained. The further increase of the metal precursor concentration led to a mixture of the orthorhombic *P*na2₁ and the tetragonal *I*̅42*d polymorphs, similar to
that observed in the *1-step* synthesis. An increase in the metal precursor concentration did not only lead to the prevalence of the tetragonal *I*42*d* polymorph but also resulted in an increased amount of Ag₂S impurity.

<figure><img src="image_5.png" /><figcaption>**Figure 3.** SEM images of the *1-step*-synthesized AgInS₂ made with varying metal precursor concentrations in water: (a) 0.1 mmol, (b) 0.5 mmol, and (c) 1 mmol; and in DES: (d) 0.5 mmol, (e) 1 mmol, and (f) 3 mmol.</figcaption></figure>

Similar to the *2-step* water-synthesized AgInS₂, the *2-step* DES-synthesized AgInS₂ samples are also suspected to be a mixture of the hexagonal *P*6₃mc polymorph and the tetragonal *I*42*d* polymorph at the low metal precursor concentration of 0.5 and 1 mmol. It should be noted that while the PXRD patterns for *P*na2₁ and *P*6₃mc are very similar, there are distinct differences: the *P*6₃mc PXRD pattern has single peaks at ~25, ~29, and ~45° 2θ, while the *P*na2₁ PXRD pattern has double (split) peaks at the same diffraction angles (2θ). Yet again, the low crystallinity, thus broader diffraction peaks, does not allow to conclude the formation of the wurtzite *P*6₃mc polymorph unambiguously.

The PXRD pattern of the 0.1 mmol *2-step* water-synthesized AgInS₂ is almost identical to that of 0.5 mmol *2-step* DES-synthesized AgInS₂. A further increase in the metal precursor concentration first led to an increase in the fraction of tetragonal *I*42*d* polymorph in the 1 mmol *2-step* DES-synthesized sample; then, the intergrowth of the *P*na2₁ and *I*42*d* polymorphs appeared at 3 mmol and 5 mmol, with the 5 mmol sample (FWHM of 0.185) being more crystalline than the 3 mmol sample (FWHM of 0.191) of the *2-step* DES-synthesis. The observed trend in the crystallinity of the *2-step* synthesis is similar to that observed in
that observed in the *1-step* synthesis. An increase in the metal precursor concentration did not only lead to the prevalence of the tetragonal I42d polymorph but also resulted in an increased amount of Ag₂S impurity.

<figure><img src="image_6.png" /><figcaption>**Figure 3.** SEM images of the *1-step*-synthesized AgInS₂ made with varying metal precursor concentrations in water: (a) 0.1 mmol, (b) 0.5 mmol, and (c) 1 mmol; and in DES: (d) 0.5 mmol, (e) 1 mmol, and (f) 3 mmol.</figcaption></figure>

Similar to the *2-step* water-synthesized AgInS₂, the *2-step* DES-synthesized AgInS₂ samples are also suspected to be a mixture of the hexagonal *P*6₃mc polymorph and the tetragonal *I*42d polymorph at the low metal precursor concentration of 0.5 and 1 mmol. It should be noted that while the PXRD patterns for *Pna*2₁ and *P*6₃mc are very similar, there are distinct differences: the *P*6₃mc PXRD pattern has single peaks at ~25, ~29, and ~45° 2θ, while the *Pna*2₁ PXRD pattern has double (split) peaks at the same diffraction angles (2θ). Yet again, the low crystallinity, thus broader diffraction peaks, does not allow to conclude the formation of the wurtzite *P*6₃mc polymorph unambiguously.

The PXRD pattern of the 0.1 mmol *2-step* water-synthesized AgInS₂ is almost identical to that of 0.5 mmol *2-step* DES-synthesized AgInS₂. A further increase in the metal precursor concentration first led to an increase in the fraction of tetragonal *I*42d polymorph in the 1 mmol *2-step* DES-synthesized sample; then, the intergrowth of the *Pna*2₁ and *I*42d polymorphs appeared at 3 mmol and 5 mmol, with the 5 mmol sample (FWHM of 0.185) being more crystalline than the 3 mmol sample (FWHM of 0.191) of the *2-step* DES-synthesis. The observed trend in the crystallinity of the *2-step* synthesis is similar to that observed in
the *1-step* synthesis, i.e., the 5 mmol sample (FWHM of 0.185) is more crystalline than the 0.5 mmol sample (FWHM of 0.468) for the DES synthesis, and the 1 mmol sample (FWHM of 0.221) is more crystalline than the 0.1 mmol sample (FWHM of 0.412) for the water synthesis. The crystallinity also improved with an increase in the molar concentration in the *2-step* synthesis.

<figure><img src="image_6.png" /><figcaption>**Figure 4.** PXRD patterns of the *2-step* synthesis of water (blue shaded region) and DES-synthesized AgInS₂ (orange shaded region), with varying concentrations of metal precursors. Diffraction peaks for the Ag₂S impurity are denoted with an asterisk (*). The theoretical PXRD patterns include ICSD 51617, representing the *I*4̅2d; ICSD 76276, representing the *P*6₃mc; and ICSD 605408, representing the *P*na2₁ polymorph.</figcaption></figure>

In contrast to the *2-step* water-synthesized AgInS₂, the *2-step* DES-synthesized AgInS₂ samples have no impurities, except the 1 mmol *2-step* DES-synthesized AgInS₂, which has a very minor Ag₂S impurity. Based on the PXRD data in Figure 4, we believe that the *2-step* synthesis is better suited for a DES rather than water.

The SEM images obtained for the *2-step* water synthesis samples are more diverse in particles arrangement and morphology than the *1-step* water synthesis samples. The 0.1 mmol *2-step* water-synthesized AgInS₂ has a plate-like morphology with a flower, petal-like arrangement. The 0.5 mmol *2-step* water-synthesized AgInS₂ has a stacked, plate-like morphology, while the 1 mmol *2-step* water-synthesized AgInS₂ has a morphology that is clustered or rock-like. In contrast, the *2-step* DES-synthesized AgInS₂ samples have a stacked, plate-like morphology, as shown in Figure 5. There is an overall significant increase of particle size with an increase in the metal precursor concentration in the DES synthesis, but not in the water synthesis.
the *1-step* synthesis, i.e., the 5 mmol sample (FWHM of 0.185) is more crystalline than the 0.5 mmol sample (FWHM of 0.468) for the DES synthesis, and the 1 mmol sample (FWHM of 0.221) is more crystalline than the 0.1 mmol sample (FWHM of 0.412) for the water synthesis. The crystallinity also improved with an increase in the molar concentration in the *2-step* synthesis.

<figure><img src="image_7.png" /><figcaption>**Figure 4.** PXRD patterns of the *2-step* synthesis of water (blue shaded region) and DES-synthesized AgInS₂ (orange shaded region), with varying concentrations of metal precursors. Diffraction peaks for the Ag₂S impurity are denoted with an asterisk (*). The theoretical PXRD patterns include ICSD 51617, representing the *I*4̄2*d; ICSD 76276, representing the *P*6₃*m;c*; and ICSD 605408, representing the *P*na2₁ polymorph.</figcaption></figure>

In contrast to the *2-step* water-synthesized AgInS₂, the *2-step* DES-synthesized AgInS₂ samples have no impurities, except the 1 mmol *2-step* DES-synthesized AgInS₂, which has a very minor Ag₂S impurity. Based on the PXRD data in Figure 4, we believe that the *2-step* synthesis is better suited for a DES rather than water.

The SEM images obtained for the *2-step* water synthesis samples are more diverse in particles arrangement and morphology than the *1-step* water synthesis samples. The 0.1 mmol *2-step* water-synthesized AgInS₂ has a plate-like morphology with a flower, petal-like arrangement. The 0.5 mmol *2-step* water-synthesized AgInS₂ has a stacked, plate-like morphology, while the 1 mmol *2-step* water-synthesized AgInS₂ has a morphology that is clustered or rock-like. In contrast, the *2-step* DES-synthesized AgInS₂ samples have a stacked, plate-like morphology, as shown in Figure 5. There is an overall significant increase of particle size with an increase in the metal precursor concentration in the DES synthesis, but not in the water synthesis.
<figure><img src="image_7.png" /><figcaption>**Figure 5.** SEM images of the 2-step-synthesized AgInS₂ made with varying metal precursor concentrations in water: (a) 0.1 mmol, (b) 0.5 mmol, and (c) 1 mmol; and in DES: (d) 1 mmol, (e) 3 mmol, and (f) 5 mmol.</figcaption></figure>

## 2.1. Scanning Transmission Electron Microscopy Study

The solution synthesis of AgInS₂ reported here always results in two polymorphs: the tetragonal I42d chalcopyrite structure and the orthorhombic Pna2₁ wurtzite-like structure. Additionally, the PXRD patterns of AgInS₂ samples (Figure 4) prepared using a 2-step heating profile and a low concentration of metal precursors (0.1 mmol for water and 0.5 mmol for DES) could be interpreted as a mixture of the tetragonal I42d and hexagonal P6₃mc wurtzite structure. We have utilized a high-resolution high-angle annular dark-field scanning transmission electron microscopy (HAADF-STEM) to address the following questions:

1. Do tetragonal I42d and orthorhombic Pna2₁ wurtzite-like polymorphs form as an intergrowth, or do they precipitate as separate particles?

2. Does the AgInS₂ polymorph with P6₃mc wurtzite structure and disorder in Ag/In cations form at lower concentrations of metal precursors and 2-step heating profile?

The HAADF-STEM image of AgInS₂ prepared via the 2-step heating profile, DES solvent route, and 0.5 mmol metal precursors concentration (see Figure 4) suggests the
<figure><img src="image_8.png" /><figcaption>**Figure 5.** SEM images of the 2-step-synthesized AgInS₂ made with varying metal precursor concentrations in water: (a) 0.1 mmol, (b) 0.5 mmol, and (c) 1 mmol; and in DES: (d) 1 mmol, (e) 3 mmol, and (f) 5 mmol.</figcaption></figure>

## 2.1. Scanning Transmission Electron Microscopy Study

The solution synthesis of AgInS₂ reported here always results in two polymorphs: the tetragonal I42d chalcopyrite structure and the orthorhombic Pna2₁ wurtzite-like structure. Additionally, the PXRD patterns of AgInS₂ samples (Figure 4) prepared using a 2-step heating profile and a low concentration of metal precursors (0.1 mmol for water and 0.5 mmol for DES) could be interpreted as a mixture of the tetragonal I42d and hexagonal P6₃mc wurtzite structure. We have utilized a high-resolution high-angle annular dark-field scanning transmission electron microscopy (HAADF-STEM) to address the following questions:

1. Do tetragonal I42d and orthorhombic Pna2₁ wurtzite-like polymorphs form as an intergrowth, or do they precipitate as separate particles?

2. Does the AgInS₂ polymorph with P6₃mc wurtzite structure and disorder in Ag/In cations form at lower concentrations of metal precursors and 2-step heating profile?

The HAADF-STEM image of AgInS₂ prepared via the 2-step heating profile, DES solvent route, and 0.5 mmol metal precursors concentration (see Figure 4) suggests the
intergrowth of two polymorphs: tetragonal I42d and orthorhombic Pna2₁ (Figure 6) with the clear phase boundary along (001)orth plane, indicated by arrows in Figure 6.

<figure><img src="image_8.png" /><figcaption>**Figure 6.** High-resolution HAADF-STEM image of AgInS₂ crystallite prepared via 2-step heating profile, 0.5 mmol metal concentration, and DES. The arrows indicate the phase boundary between orthorhombic and tetragonal (in blue) polymorphs.</figcaption></figure>

We further investigated the structure of the presumed *P*6₃mc wurtzite polymorph. The high-intensity diffraction spots in the electron diffraction (ED) patterns collected in the *ab*-plane and along the *c*-axis of the wurtzite structure can be indexed in a hexagonal unit cell (Figure 7: top, yellow), corresponding to the wurtzite structure. However, there are plenty of low-intensity reflections that cannot be indexed using the wurtzite cell but can be indexed in the *P*-orthorhombic cell with quadrupled volume. Therefore, the structure is better described as pseudo-wurtzite since the deviation from ideal hexagonal symmetry is observed. The HAADF-STEM images and simulated images of the structure further support this conclusion. The HAADF-STEM image in the *ab*-plane (Figure 7: middle right) supports the hexagonal in-plane arrangement of the Ag and In cations, while a variation of the contrast, seen in the lower magnification HAADF-STEM image, suggests the non-uniform distribution of Ag and In cations in the atomic columns, e.g., clustering. The Fast Fourier Transform (FFT) pattern (not shown here) includes the weak diffraction spots that are forbidden in the simple hexagonal wurtzite cell, further supporting the pseudo-wurtzite structure. All weak diffraction spots presented in the [001]orth ED pattern can be indexed based on the orthorhombic *P*na2₁ structure. The simulated image of the structure performed along [001]ort and [010]ort directions (see insert Figure 7) strongly supports the orthorhombic structure with the clear pseudo-hexagonal symmetry. Importantly, the performed EDX-STEM elemental mapping (Figure 7 bottom panel) demonstrates the
intergrowth of two polymorphs: tetragonal I42d and orthorhombic Pna2₁ (Figure 6) with the clear phase boundary along (001)orth plane, indicated by arrows in Figure 6.

<figure><img src="image_9.png" /><figcaption>**Figure 6.** High-resolution HAADF-STEM image of AgInS₂ crystallite prepared via 2-step heating profile, 0.5 mmol metal concentration, and DES. The arrows indicate the phase boundary between orthorhombic and tetragonal (in blue) polymorphs.</figcaption></figure>

We further investigated the structure of the presumed *P*6₃mc wurtzite polymorph. The high-intensity diffraction spots in the electron diffraction (ED) patterns collected in the *ab*-plane and along the *c*-axis of the wurtzite structure can be indexed in a hexagonal unit cell (Figure 7: top, yellow), corresponding to the wurtzite structure. However, there are plenty of low-intensity reflections that cannot be indexed using the wurtzite cell but can be indexed in the *P*-orthorhombic cell with quadrupled volume. Therefore, the structure is better described as pseudo-wurtzite since the deviation from ideal hexagonal symmetry is observed. The HAADF-STEM images and simulated images of the structure further support this conclusion. The HAADF-STEM image in the *ab*-plane (Figure 7: middle right) supports the hexagonal in-plane arrangement of the Ag and In cations, while a variation of the contrast, seen in the lower magnification HAADF-STEM image, suggests the non-uniform distribution of Ag and In cations in the atomic columns, e.g., clustering. The Fast Fourier Transform (FFT) pattern (not shown here) includes the weak diffraction spots that are forbidden in the simple hexagonal wurtzite cell, further supporting the pseudo-wurtzite structure. All weak diffraction spots presented in the [001]orth ED pattern can be indexed based on the orthorhombic *P*na2₁ structure. The simulated image of the structure performed along [001]ort and [010]ort directions (see insert Figure 7) strongly supports the orthorhombic structure with the clear pseudo-hexagonal symmetry. Importantly, the performed EDX-STEM elemental mapping (Figure 7 bottom panel) demonstrates the
homogeneous distribution of all elements with a nominal composition close to AgInS₂. The
appearance of nanoparticles that are free from In (showing as more red in the bottom panel
of Figure 7) is in agreement with the presence of the small Ag₂S impurity.

<figure><img src="image_9.png" /></figure>

**Figure 7.** (Top and Middle, Left) High-resolution HAADF-STEM images and corresponding electron diffraction (ED) patterns of the two main zones of the (pseudo)-wurtzite AgInS₂ structure: top panel, [001] and middle panel, [010]ort/[100]hex. High-intensity diffraction spots can be indexed using hexagonal wurtzite structure (P6₃mc, yellow). All of the diffraction spots, including those with lower intensity can be indexed using the orthorhombic wurtzite-like structure (Pna2₁ space group). **Top and Middle, Right:** Magnified high-resolution HAADF-STEM images of the two main
homogeneous distribution of all elements with a nominal composition close to AgInS₂. The
appearance of nanoparticles that are free from In (showing as more red in the bottom panel
of Figure 7) is in agreement with the presence of the small Ag₂S impurity.

<figure><img src="image_10.png" /></figure>

**Figure 7.** (Top and Middle, Left) High-resolution HAADF-STEM images and corresponding electron diffraction (ED) patterns of the two main zones of the (pseudo)-wurtzite AgInS₂ structure: top panel, [001] and middle panel, [010]ort/[100]hex. High-intensity diffraction spots can be indexed using hexagonal wurtzite structure (P6₃mc, yellow). All of the diffraction spots, including those with lower intensity can be indexed using the orthorhombic wurtzite-like structure (Pna2₁ space group). **Top and Middle, Right:** Magnified high-resolution HAADF-STEM images of the two main
zones and simulated images based on orthorhombic wurtzite-like structure (Pna2₁ space group) as inserts. **Bottom:** Images of the EDX-STEM elemental mapping for Ag L(red), In L (green), S K (blue), and an overlapping color image.

Therefore, our study by ED and HAADF-STEM confirms the formation of an inter-growth of two AgInS₂ polymorphs, tetragonal I̅42d and orthorhombic Pna2₁, within the same particle. Additionally, STEM clearly reveals that the previously reported wurtzite structure is best described as orthorhombic with pseudo-hexagonal symmetry. Thus, the synthesis using the 2-step profile and low concentrations of metal precursors results in the intergrowth of two polymorphs, tetragonal and pseudo-hexagonal wurtzite-like structures, with the latter best described as an orthorhombic structure.

## 2.2. High-Temperature PXRD

The 0.5 mmol 2-step DES-synthesized AgInS₂ represents a metastable intergrowth of the two polymorphs–tetragonal and pseudo-hexagonal (best described as orthorhombic). We further investigated the thermal transformation of this metastable intergrowth by collecting the high-temperature synchrotron in situ PXRD data (HT–PXRD) on the 0.5 mmol 2-step DES-synthesized AgInS₂. The data was collected on the powdered sample upon heating and cooling, as shown in Figure 8. The HT–PXRD data shows an intergrowth of the pseudo-hexagonal wurtzite-like polymorph and the I̅42d polymorph at room temperature. While the fraction of the I̅42d polymorph increased upon heating, a transformation of the pseudo-hexagonal polymorph to orthorhombic Pna2₁ happened between 355 and 380 °C. The combination of Pna2₁ and I̅42d polymorphs persisted until 700 °C, where the peaks belonging to the Pna2₁ polymorph began to increase in intensity and at 790 °C the orthorhombic phase was the only polymorph. The Pna2₁ AgInS₂ remained the only crystalline phase upon heating until 863 °C, when the peaks belonging to the AgIn₅S₈ began to appear in the HT–PXRD pattern. At 890 °C AgIn₅S₈ was the only crystalline phase, suggesting that Ag₂S and In₂S₃ were molten:

$$12\text{AgInS}_{2}(\text{s}) \xrightarrow{\text{decomposition}} 2\text{AgIn}_{5}\text{S}_{8}(\text{s}) + 5\text{Ag}_{2}\text{S}_{(\text{melt})} + \text{In}_{2}\text{S}_{3}(\text{melt}) \quad (1)$$

<figure><img src="image_10.png" /><figcaption>Figure 8. HT–PXRD data of 0.5 mmol the 2-step DES-synthesized AgInS₂ upon heating and cooling.</figcaption></figure>
zones and simulated images based on orthorhombic wurtzite-like structure (Pna2₁ space group) as inserts. **Bottom:** Images of the EDX-STEM elemental mapping for Ag L(red), In L (green), S K (blue), and an overlapping color image.

Therefore, our study by ED and HAADF-STEM confirms the formation of an inter-growth of two AgInS₂ polymorphs, tetragonal I̅42d and orthorhombic Pna2₁, within the same particle. Additionally, STEM clearly reveals that the previously reported wurtzite structure is best described as orthorhombic with pseudo-hexagonal symmetry. Thus, the synthesis using the 2-step profile and low concentrations of metal precursors results in the intergrowth of two polymorphs, tetragonal and pseudo-hexagonal wurtzite-like structures, with the latter best described as an orthorhombic structure.

## 2.2. High-Temperature PXRD

The 0.5 mmol 2-step DES-synthesized AgInS₂ represents a metastable intergrowth of the two polymorphs–tetragonal and pseudo-hexagonal (best described as orthorhombic). We further investigated the thermal transformation of this metastable intergrowth by collecting the high-temperature synchrotron in situ PXRD data (HT–PXRD) on the 0.5 mmol 2-step DES-synthesized AgInS₂. The data was collected on the powdered sample upon heating and cooling, as shown in Figure 8. The HT–PXRD data shows an intergrowth of the pseudo-hexagonal wurtzite-like polymorph and the I̅42d polymorph at room temperature. While the fraction of the I̅42d polymorph increased upon heating, a transformation of the pseudo-hexagonal polymorph to orthorhombic Pna2₁ happened between 355 and 380 °C. The combination of Pna2₁ and I̅42d polymorphs persisted until 700 °C, where the peaks belonging to the Pna2₁ polymorph began to increase in intensity and at 790 °C the orthorhombic phase was the only polymorph. The Pna2₁ AgInS₂ remained the only crystalline phase upon heating until 863 °C, when the peaks belonging to the AgIn₅S₈ began to appear in the HT–PXRD pattern. At 890 °C AgIn₅S₈ was the only crystalline phase, suggesting that Ag₂S and In₂S₃ were molten:

$$12\text{AgInS}_{2}(\text{s}) \xrightarrow{\text{decomposition}} 2\text{AgIn}_{5}\text{S}_{8}(\text{s}) + 5\text{Ag}_{2}\text{S}_{(\text{melt})} + \text{In}_{2}\text{S}_{3}(\text{melt}) \quad (1)$$

<figure><img src="image_11.png" /><figcaption>Figure 8. HT–PXRD data of 0.5 mmol the 2-step DES-synthesized AgInS₂ upon heating and cooling.</figcaption></figure>
Upon cooling, AgIn<sub>5</sub>S<sub>8</sub> reacted with the molten Ag<sub>2</sub>S and In<sub>2</sub>S<sub>3</sub> and gave the Pna2<sub>1</sub> polymorph of AgInS<sub>2</sub>. It is important to note the high-temperature orthorhombic polymorph formed, albeit as a minor phase, at synthesis temperatures, well below the transition between tetragonal I42d and orthorhombic Pna2<sub>1</sub> polymorphs.

## 2.3. Diffuse Reflectance

The effect of the synthesis conditions on the optical properties of the synthesized samples was investigated by diffuse reflectance using a UV-Vis-NIR spectrophotometer. In order to obtain the values of the bandgap, data was converted into Tauc plot, e.g. $(a \times \hnu)^r$ vs. $\hnu$, where *a* is proportional to the absorption coefficient, $\hnu$ is the excitation energy in eV, and *r* = 2 is for the direct allowed transitions. The bandgap was determined as the intercept of a tangent line and a baseline, as shown in Figure 9d. The additional absorption edge at ~1.0 eV was attributed to the Ag<sub>2</sub>S impurity. Three trends became apparent; firstly, the 2-step synthesis resulted in AgInS<sub>2</sub> with slightly smaller bandgaps for the same precursor concentration and solvent used; secondly, the increase in the metal precursor concentrations led to the slight increase in the bandgap values; and, lastly, the bandgap values for the AgInS<sub>2</sub> synthesized using the DES were overall slightly higher than that for the water synthesis.

<figure><img src="image_11.png" /><figcaption>**Figure 9.** Tauc plots for AgInS<sub>2</sub> obtained via (a) 1-step and (b) 2-step synthesis; (c) the PXRD pattern of high-temperature Pna2<sub>1</sub> orthorhombic AgInS<sub>2</sub> polymorph, synthesized via a high-temperature route; and (d) Tauc plot of high-temperature Pna2<sub>1</sub> orthorhombic AgInS<sub>2</sub> polymorph, synthesized via high-temperature route.</figcaption></figure>

The reported values of the bandgaps span the range of 1.86–1.87 eV for the tetragonal I42d polymorph (chalcopyrite structure) and 1.96–1.98 eV for the Pna2₁ orthorhombic
Upon cooling, AgIn<sub>5</sub>S<sub>8</sub> reacted with the molten Ag<sub>2</sub>S and In<sub>2</sub>S<sub>3</sub> and gave the Pna2<sub>1</sub> polymorph of AgInS<sub>2</sub>. It is important to note the high-temperature orthorhombic polymorph formed, albeit as a minor phase, at synthesis temperatures, well below the transition between tetragonal I42d and orthorhombic Pna2<sub>1</sub> polymorphs.

## 2.3. Diffuse Reflectance

The effect of the synthesis conditions on the optical properties of the synthesized samples was investigated by diffuse reflectance using a UV-Vis-NIR spectrophotometer. In order to obtain the values of the bandgap, data was converted into Tauc plot, e.g. $(a \times \hnu)^r$ vs. $\hnu$, where *a* is proportional to the absorption coefficient, $\hnu$ is the excitation energy in eV, and *r* = 2 is for the direct allowed transitions. The bandgap was determined as the intercept of a tangent line and a baseline, as shown in Figure 9d. The additional absorption edge at ~1.0 eV was attributed to the Ag<sub>2</sub>S impurity. Three trends became apparent; firstly, the 2-step synthesis resulted in AgInS<sub>2</sub> with slightly smaller bandgaps for the same precursor concentration and solvent used; secondly, the increase in the metal precursor concentrations led to the slight increase in the bandgap values; and, lastly, the bandgap values for the AgInS<sub>2</sub> synthesized using the DES were overall slightly higher than that for the water synthesis.

<figure><img src="image_12.png" /><figcaption>**Figure 9.** Tauc plots for AgInS<sub>2</sub> obtained via (a) 1-step and (b) 2-step synthesis; (c) the PXRD pattern of high-temperature Pna2<sub>1</sub> orthorhombic AgInS<sub>2</sub> polymorph, synthesized via a high-temperature route; and (d) Tauc plot of high-temperature Pna2<sub>1</sub> orthorhombic AgInS<sub>2</sub> polymorph, synthesized via high-temperature route.</figcaption></figure>

The reported values of the bandgaps span the range of 1.86–1.87 eV for the tetragonal I42d polymorph (chalcopyrite structure) and 1.96–1.98 eV for the Pna2₁ orthorhombic
(wurtzite-like structure) polymorph [17,20,21], while larger values of the bandgap were measured for the AgInS₂ nanoparticles due to the quantum confinement effect and Ag/In non-stoichiometry [24,25]. The solution synthesis in either the water or the DES results in AgInS₂ with the bandgap on the slightly lower side compared to the literature, which we tentatively attribute to the formation of intergrowth between the tetragonal and orthorhombic polymorphs.

We also compared the bandgap of the polymorph mixture obtained using the solution synthesis with the bandgap of the orthorhombic Pna2₁ polymorph, which was synthesized by high-temperature annealing (at 800 °C at 10 °C/min for 30 min) of the 0.1 mmol 2-step water-synthesized AgInS₂ (Figure 9c,d). The high-temperature-synthesized Pna2₁ orthorhombic polymorph is highly crystalline and has a bandgap of 1.94 eV, which is comparable to the previously reported values [17,20,21].

### 3. Conclusions

We have studied the solution microwave-assisted synthesis of AgInS₂ from two solvents—water and an eutectic mixture of choline chloride and thiourea (a deep eutectic solvent). AgInS₂ was previously reported to have four polymorphic modifications. According to the literature data, the tetragonal I42d (chalcopyrite structure) is the thermodynamically stable polymorph at room-temperature, which transforms into a high-temperature orthorhombic (wurtzite-like) polymorph at ~620 °C. The microwave-assisted solution synthesis from either the water or the DES resulted in a metastable mixture of tetragonal and orthorhombic polymorphs of AgInS₂, with the tetragonal I42d being prevalent. We also investigated how the fraction and crystallinity of the polymorphs formed can be controlled by varying the heating profile, solvent type, and metal precursor concentration. Overall, the increase in the metal precursor concentrations improved the crystallinity of the polymorphic intergrowth, while the 2-step microwave heating profile was better suited for the DES synthesis because the binary sulfides impurities were eliminated. We further studied the possible mechanism of the AgInS₂ formation from the solution via the microwave-assisted synthesis and ruled out the partial cation exchange between the crystalline binary sulfide and a cation in the solution as a possible mechanism.

The PXRD data of the AgInS₂ samples prepared via the 2-step heating profile and low concentrations of metal precursors have initially suggested the possible formation of hexagonal polymorph with wurtzite structure and Ag/In mixed occupied cation positions. The state-of-the-art study by scanning transmission electron microscopy (STEM) revealed that the long thought wurtzite polymorph has, indeed, pseudo-hexagonal symmetry, and its structure is best described as an orthorhombic structure alike to the high-temperature Pna2₁ polymorph. The STEM study further revealed that the solution synthesis from the DES resulted in the intergrowth of tetragonal and orthorhombic polymorphs within the same particle, thus resulting in the metastable product.

The bandgaps of the solution synthesized AgInS₂ are similar, albeit a bit lower compared to the previously reported values for both the tetragonal and orthorhombic polymorphs.

### 4. Materials and Methods

Silver nitrate, AgNO₃ (Alfa Aesar, 99.9+%); indium chloride, InCl₃·yH₂O (Alfa Aesar, 99.9+%); thiourea, CH₄N₂S (Acros 99+%); choline chloride, (CH₃)₃N(Cl)CH₂CH₂OH (Sigma-Aldrich, 98%), and deionized (DI) water were used as received.

AgInS₂ was synthesized in either DI water or Deep Eutectic Solvent (DES). For the DI water synthesis, powders of AgNO₃, InCl₃·yH₂O, and CH₄N₂S were weighted in x:x:5 molar ratio (where x = 0.1, 0.5 and 1 mmols), respectively, loaded into a microwave tube with 6 mL of DI water, and heated in a microwave reactor with a 1-step or 2-step heating profile. For the DES synthesis, powders of AgNO₃ and InCl₃·yH₂O were weighted in x:x molar ratio (where x = 0.5, 1, 3 and 5 mmol). After that, approximately 4 g of thiourea and 3.59 g of choline chloride were added to the metal precursors in a microwave tube and heated in a Monowave 400 microwave reactor (Anton Paar) with a 1-step or 2-step heating
(wurtzite-like structure) polymorph [17,20,21], while larger values of the bandgap were measured for the AgInS₂ nanoparticles due to the quantum confinement effect and Ag/In non-stoichiometry [24,25]. The solution synthesis in either the water or the DES results in AgInS₂ with the bandgap on the slightly lower side compared to the literature, which we tentatively attribute to the formation of intergrowth between the tetragonal and orthorhombic polymorphs.

We also compared the bandgap of the polymorph mixture obtained using the solution synthesis with the bandgap of the orthorhombic Pna2₁ polymorph, which was synthesized by high-temperature annealing (at 800 °C at 10 °C/min for 30 min) of the 0.1 mmol 2-step water-synthesized AgInS₂ (Figure 9c,d). The high-temperature-synthesized Pna2₁ orthorhombic polymorph is highly crystalline and has a bandgap of 1.94 eV, which is comparable to the previously reported values [17,20,21].

### 3. Conclusions

We have studied the solution microwave-assisted synthesis of AgInS₂ from two solvents—water and an eutectic mixture of choline chloride and thiourea (a deep eutectic solvent). AgInS₂ was previously reported to have four polymorphic modifications. According to the literature data, the tetragonal I42d (chalcopyrite structure) is the thermodynamically stable polymorph at room-temperature, which transforms into a high-temperature orthorhombic (wurtzite-like) polymorph at ~620 °C. The microwave-assisted solution synthesis from either the water or the DES resulted in a metastable mixture of tetragonal and orthorhombic polymorphs of AgInS₂, with the tetragonal I42d being prevalent. We also investigated how the fraction and crystallinity of the polymorphs formed can be controlled by varying the heating profile, solvent type, and metal precursor concentration. Overall, the increase in the metal precursor concentrations improved the crystallinity of the polymorphic intergrowth, while the 2-step microwave heating profile was better suited for the DES synthesis because the binary sulfides impurities were eliminated. We further studied the possible mechanism of the AgInS₂ formation from the solution via the microwave-assisted synthesis and ruled out the partial cation exchange between the crystalline binary sulfide and a cation in the solution as a possible mechanism.

The PXRD data of the AgInS₂ samples prepared via the 2-step heating profile and low concentrations of metal precursors have initially suggested the possible formation of hexagonal polymorph with wurtzite structure and Ag/In mixed occupied cation positions. The state-of-the-art study by scanning transmission electron microscopy (STEM) revealed that the long thought wurtzite polymorph has, indeed, pseudo-hexagonal symmetry, and its structure is best described as an orthorhombic structure alike to the high-temperature Pna2₁ polymorph. The STEM study further revealed that the solution synthesis from the DES resulted in the intergrowth of tetragonal and orthorhombic polymorphs within the same particle, thus resulting in the metastable product.

The bandgaps of the solution synthesized AgInS₂ are similar, albeit a bit lower compared to the previously reported values for both the tetragonal and orthorhombic polymorphs.

### 4. Materials and Methods

Silver nitrate, AgNO₃ (Alfa Aesar, 99.9+%); indium chloride, InCl₃·yH₂O (Alfa Aesar, 99.9+%); thiourea, CH₄N₂S (Acros 99+%); choline chloride, (CH₃)₃N(Cl)CH₂CH₂OH (Sigma-Aldrich, 98%), and deionized (DI) water were used as received.

AgInS₂ was synthesized in either DI water or Deep Eutectic Solvent (DES). For the DI water synthesis, powders of AgNO₃, InCl₃·yH₂O, and CH₄N₂S were weighted in x:x:5 molar ratio (where x = 0.1, 0.5 and 1 mmols), respectively, loaded into a microwave tube with 6 mL of DI water, and heated in a microwave reactor with a 1-step or 2-step heating profile. For the DES synthesis, powders of AgNO₃ and InCl₃·yH₂O were weighted in x:x molar ratio (where x = 0.5, 1, 3 and 5 mmol). After that, approximately 4 g of thiourea and 3.59 g of choline chloride were added to the metal precursors in a microwave tube and heated in a Monowave 400 microwave reactor (Anton Paar) with a 1-step or 2-step heating
profile. The resulting mixture of AgInS₂ and solvent from either the water or DES synthesis was then washed with water by sonication and centrifuged several times. Then, it was further washed with ethanol and centrifuged several times until the supernatant is clear. The AgInS₂ was then dried in a static vacuum overnight.

**1-step** heating profile: The loaded microwave tube was placed in a Monowave 400 mi-crowave reactor and heated to 180 °C for 8 min. It then dwelled for 2 h. The resulting mixture was then cooled to room temperature.

**2-step** heating profile: The loaded microwave tube was placed in a Monowave 400 mi-crowave reactor and heated to 80 °C for 5 min and dwelled for 20 min. The reaction mixture was then quickly (~1 min) heated to 180 °C and dwelled for 1 h. The resulting mixture was cooled to room temperature.

# 5. Characterization

## 5.1. Powder X-ray Diffraction

Samples were analyzed by powder X-ray diffraction (PXRD) using a Rigaku Miniflex 600 diffractometer with Cu Kα radiation (λ = 1.54051 Å). Measurement was carried out on a silicon, zero-background holder at room temperature in air. The powder pattern was collected in 0.02° steps increment at a rate of 10°/minute. Phase identification was performed using the Match! 2.0 software [26]. The Full width at half maximum (FWHM) was determined using the PDXL software [27].

## 5.2. Diffuse Reflectance UV-Vis Spectroscopy

The diffuse reflectance of the powdered samples was collected on a Perkin Elmer Lambda 1050+ UV/Vis/NIR spectrophotometer in reflectance mode. The instrument was equipped with a 150 mm Spectralon-coated integrating sphere. We loaded finely ground samples into a powder holder, which had a lens. The samples were pressed against the lens and held in place by a press and a spring within the holder. We then placed the holder at the reflectance port, while the specular port was left open. The Iris aperture was adjusted so that the sample beam was focused only on the samples. A sample holder containing a lens and Spectralon reference standard was used as a blank.

## 5.3. Scanning Electron Microscopy and Energy Dispersive Spectroscopy

Elemental analysis was performed using a JEOL JSM-IT200 scanning electron micro-scope (SEM) equipped with a JEOL energy-dispersive X-ray (EDX) analysis system with a silicon drift detector. Powder samples were adhered to aluminum stubs using carbon tape and then placed into an aluminum holder for insertion into the SEM. Samples were oriented perpendicular to the beam and analyzed using a 15 kV accelerating voltage with an accumulation time of 60 s.

## 5.4. High-Temperature Synchrotron Powder X-ray Diffraction (HT-PXRD)

High temperature in situ synchrotron powder diffraction data were collected for AgInS₂ at beamline 17-BM Advanced Photon Source (APS) at Argonne National Labora-tory, with a wavelength of 0.24158 Å. The powdered sample of AgInS₂ was loaded into a 0.7 mm outer diameter silica capillary, which was sealed under vacuum. The sealed tube was then inserted into a second silica tube of 0.9 mm inner diameter and 1.1 mm outer diameter, and this second tube was mounted on a sample stage featuring two micro-heaters and a thermocouple, which was placed close to the area being measured. Details of the experimental setup can be found elsewhere [28]. Data were collected from room tempera-ture to 895 °C at the rate of 15 °C/min, and also upon cooling. Diffraction patterns were analyzed using Match! 2.0 software [26].

## 5.5. Differential Scanning Calorimetry

The DSC/TGA experiment was performed using a Netzsch STA449 F1 Jupiter. 5 mg of the powdered sample (1-step water-synthesized In₂S₃) was loaded into a pan-type alumina
profile. The resulting mixture of AgInS₂ and solvent from either the water or DES synthesis was then washed with water by sonication and centrifuged several times. Then, it was further washed with ethanol and centrifuged several times until the supernatant is clear. The AgInS₂ was then dried in a static vacuum overnight.

**1-step** heating profile: The loaded microwave tube was placed in a Monowave 400 mi-crowave reactor and heated to 180 °C for 8 min. It then dwelled for 2 h. The resulting mixture was then cooled to room temperature.

**2-step** heating profile: The loaded microwave tube was placed in a Monowave 400 mi-crowave reactor and heated to 80 °C for 5 min and dwelled for 20 min. The reaction mixture was then quickly (~1 min) heated to 180 °C and dwelled for 1 h. The resulting mixture was cooled to room temperature.

# 5. Characterization

## 5.1. Powder X-ray Diffraction

Samples were analyzed by powder X-ray diffraction (PXRD) using a Rigaku Miniflex 600 diffractometer with Cu Kα radiation (λ = 1.54051 Å). Measurement was carried out on a silicon, zero-background holder at room temperature in air. The powder pattern was collected in 0.02° steps increment at a rate of 10°/minute. Phase identification was performed using the Match! 2.0 software [26]. The Full width at half maximum (FWHM) was determined using the PDXL software [27].

## 5.2. Diffuse Reflectance UV-Vis Spectroscopy

The diffuse reflectance of the powdered samples was collected on a Perkin Elmer Lambda 1050+ UV/Vis/NIR spectrophotometer in reflectance mode. The instrument was equipped with a 150 mm Spectralon-coated integrating sphere. We loaded finely ground samples into a powder holder, which had a lens. The samples were pressed against the lens and held in place by a press and a spring within the holder. We then placed the holder at the reflectance port, while the specular port was left open. The Iris aperture was adjusted so that the sample beam was focused only on the samples. A sample holder containing a lens and Spectralon reference standard was used as a blank.

## 5.3. Scanning Electron Microscopy and Energy Dispersive Spectroscopy

Elemental analysis was performed using a JEOL JSM-IT200 scanning electron micro-scope (SEM) equipped with a JEOL energy-dispersive X-ray (EDX) analysis system with a silicon drift detector. Powder samples were adhered to aluminum stubs using carbon tape and then placed into an aluminum holder for insertion into the SEM. Samples were oriented perpendicular to the beam and analyzed using a 15 kV accelerating voltage with an accumulation time of 60 s.

## 5.4. High-Temperature Synchrotron Powder X-ray Diffraction (HT-PXRD)

High temperature in situ synchrotron powder diffraction data were collected for AgInS₂ at beamline 17-BM Advanced Photon Source (APS) at Argonne National Labora-tory, with a wavelength of 0.24158 Å. The powdered sample of AgInS₂ was loaded into a 0.7 mm outer diameter silica capillary, which was sealed under vacuum. The sealed tube was then inserted into a second silica tube of 0.9 mm inner diameter and 1.1 mm outer diameter, and this second tube was mounted on a sample stage featuring two micro-heaters and a thermocouple, which was placed close to the area being measured. Details of the experimental setup can be found elsewhere [28]. Data were collected from room tempera-ture to 895 °C at the rate of 15 °C/min, and also upon cooling. Diffraction patterns were analyzed using Match! 2.0 software [26].

## 5.5. Differential Scanning Calorimetry

The DSC/TGA experiment was performed using a Netzsch STA449 F1 Jupiter. 5 mg of the powdered sample (1-step water-synthesized In₂S₃) was loaded into a pan-type alumina
(Al₂O₃) crucible with an alumina cover. The sample was heated from 40 to 200, or 500 °C, and, subsequently, cooled to 50 °C, with a rate of 10 °C/min under a constant argon gas flow.

### 5.6. Scanning Transmission Electron Microscopy (STEM) and Electron Diffraction

HAADF-STEM imaging and ED studies were performed using JEM ARM200F cold FEG double aberration corrected microscope operated at 200 kV, equipped with a large angle CENTURIO EDX detector, Orius CCD camera, and Quantum GIF. Samples for STEM were prepared by mechanical grinding of material in an agate mortar, adding ethanol and depositing obtained suspension on the Cu holey carbon grid. HAADF-STEM image simulation was done using JEMS Software developed by P. Stadelmann. The 0.5 mmol 2-step DES-synthesized AgInS₂ was used for STEM analysis.

**Supplementary Materials:** The following supporting information can be downloaded at: https://www.mdpi.com/article/10.3390/molecules27061815/s1, Figure S1: PXRD pattern of 1-step and 2-step synthesized In₂S₃ in both water and DES; Figure S2: (a) DSC/TGA data of water synthesized In₂S₃ at 500 °C (b) PXRD pattern of water synthesized In₂S₃ before and after DSC at 200 °C and 500 °C; Figure S3: PXRD pattern of (a) 1-step water synthesized In₂S₃; (b) the instantaneously formed product of a reaction of pre-made In₂S₃ with aqueous AgNO₃ solution; (c) the Ag₂S product obtained from the metathesis reaction of In₂S₃ with a twice concentrated aqueous AgNO₃ solution at room temperature which was left undisturbed for 2 days.

**Author Contributions:** Conceptualization, project supervision, resources, J.V.Z.; methodology, formal analysis, writing—original draft preparation, visualization, A.N.A.; investigation, data collection, curation, and validation, formal analysis, A.N.A., R.A.E., T.C., O.I.L. All authors have read and agreed to the published version of the manuscript.

**Funding:** This research was funded by J.V.Z. startup funds from Iowa State University. Use of the Advanced Photon Source at Argonne National Laboratory was supported by the U. S. Department of Energy, Office of Science, and Office of Basic Energy Sciences, under contract no. DE-AC02-06CH11357.

**Data Availability Statement:** The data presented in this study are available in article and Supplementary Materials, and are also available on request from the corresponding author.

**Acknowledgments:** We thank Kirill Kovnir (Department of Chemistry, Iowa State University, and Ames Laboratory) for the access to the PXRD diffractometer; Brett Boote (Chemical Instrumentation facility, Iowa State University) for the help with the DSC/TGA instrument and the SEM.

**Conflicts of Interest:** The authors declare no conflict of interest.

## References

1. Abbott, A.P.; Boothby, D.; Capper, G.; Davies, D.L.; Rasheed, R.K. Deep Eutectic Solvents Formed between Choline Chloride and Carboxylic Acids: Versatile Alternatives to Ionic Liquids. *J. Am. Chem. Soc.* **2004**, *126*, 9142–9147. [CrossRef] [PubMed]

2. Abbott, A.P.; Capper, G.; Davies, D.L.; Rasheed, R.K.; Tambyrajah, V. Novel solvent properties of choline chloride/urea mixtures. *Chem. Commun.* **2003**, 70–71. [CrossRef] [PubMed]

3. Zhang, Q.H.; Vigier, K.D.; Royer, S.; Jerome, F. Deep eutectic solvents: Syntheses, properties and applications. *Chem. Soc. Rev.* **2012**, *41*, 7108–7146. [CrossRef]

4. Abbott, A.P.; Capper, G.; Davies, D.L.; McKenzie, K.J.; Obi, S.U. Solubility of Metal Oxides in Deep Eutectic Solvents Based on Choline Chloride. *J. Chem. Eng. Data* **2006**, *51*, 1280–1282. [CrossRef]

5. Hong, S.K.; Doughty, R.M.; Osterloh, F.E.; Zaikina, J.V. Deep eutectic solvent route synthesis of zinc and copper vanadate n-type semiconductors-mapping oxygen vacancies and their effect on photovoltage. *J. Mater. Chem. A* **2019**, *7*, 12303–12316. [CrossRef]

6. Hong, S.; Burkhow, S.J.; Doughty, R.M.; Cheng, Y.; Ryan, B.J.; Mantravadi, A.; Roling, L.T.; Panthani, M.G.; Osterloh, F.E.; Smith, E.A.; et al. Local Structural Disorder in Metavanadates MV₂O₆ (M = Zn and Cu) Synthesized by the Deep Eutectic Solvent Route: Photoactive Oxides with Oxygen Vacancies. *Chem. Mater.* **2021**, *33*, 1667–1682. [CrossRef]

7. Boston, R.; Foeller, P.Y.; Sinclair, D.C.; Reaney, I.M. Synthesis of Barium Titanate Using Deep Eutectic Solvents. *Inorg. Chem.* **2017**, *56*, 542–547. [CrossRef]

8. Thorat, G.M.; Jadhav, H.S.; Roy, A.; Chung, W.J.; Seo, J.G. Dual Role of Deep Eutectic Solvent as a Solvent and Template for the Synthesis of Octahedral Cobalt Vanadate for an Oxygen Evolution Reaction. *ACS Sustain. Chem. Eng.* **2018**, *6*, 16255–16266. [CrossRef]
(Al₂O₃) crucible with an alumina cover. The sample was heated from 40 to 200, or 500 °C, and, subsequently, cooled to 50 °C, with a rate of 10 °C/min under a constant argon gas flow.

### 5.6. Scanning Transmission Electron Microscopy (STEM) and Electron Diffraction

HAADF-STEM imaging and ED studies were performed using JEM ARM200F cold FEG double aberration corrected microscope operated at 200 kV, equipped with a large angle CENTURIO EDX detector, Orius CCD camera, and Quantum GIF. Samples for STEM were prepared by mechanical grinding of material in an agate mortar, adding ethanol and depositing obtained suspension on the Cu holey carbon grid. HAADF-STEM image simulation was done using JEMS Software developed by P. Stadelmann. The 0.5 mmol 2-step DES-synthesized AgInS₂ was used for STEM analysis.

**Supplementary Materials:** The following supporting information can be downloaded at: https://www.mdpi.com/article/10.3390/molecules27061815/s1, Figure S1: PXRD pattern of 1-step and 2-step synthesized In₂S₃ in both water and DES; Figure S2: (a) DSC/TGA data of water synthesized In₂S₃ at 500 °C (b) PXRD pattern of water synthesized In₂S₃ before and after DSC at 200 °C and 500 °C; Figure S3: PXRD pattern of (a) 1-step water synthesized In₂S₃; (b) the instantaneously formed product of a reaction of pre-made In₂S₃ with aqueous AgNO₃ solution; (c) the Ag₂S product obtained from the metathesis reaction of In₂S₃ with a twice concentrated aqueous AgNO₃ solution at room temperature which was left undisturbed for 2 days.

**Author Contributions:** Conceptualization, project supervision, resources, J.V.Z.; methodology, formal analysis, writing—original draft preparation, visualization, A.N.A.; investigation, data collection, curation, and validation, formal analysis, A.N.A., R.A.E., T.C., O.I.L. All authors have read and agreed to the published version of the manuscript.

**Funding:** This research was funded by J.V.Z. startup funds from Iowa State University. Use of the Advanced Photon Source at Argonne National Laboratory was supported by the U. S. Department of Energy, Office of Science, and Office of Basic Energy Sciences, under contract no. DE-AC02-06CH11357.

**Data Availability Statement:** The data presented in this study are available in article and Supplementary Materials, and are also available on request from the corresponding author.

**Acknowledgments:** We thank Kirill Kovnir (Department of Chemistry, Iowa State University, and Ames Laboratory) for the access to the PXRD diffractometer; Brett Boote (Chemical Instrumentation facility, Iowa State University) for the help with the DSC/TGA instrument and the SEM.

**Conflicts of Interest:** The authors declare no conflict of interest.

## References

1. Abbott, A.P.; Boothby, D.; Capper, G.; Davies, D.L.; Rasheed, R.K. Deep Eutectic Solvents Formed between Choline Chloride and Carboxylic Acids: Versatile Alternatives to Ionic Liquids. *J. Am. Chem. Soc.* **2004**, *126*, 9142–9147. [CrossRef] [PubMed]

2. Abbott, A.P.; Capper, G.; Davies, D.L.; Rasheed, R.K.; Tambyrajah, V. Novel solvent properties of choline chloride/urea mixtures. *Chem. Commun.* **2003**, 70–71. [CrossRef] [PubMed]

3. Zhang, Q.H.; Vigier, K.D.; Royer, S.; Jerome, F. Deep eutectic solvents: Syntheses, properties and applications. *Chem. Soc. Rev.* **2012**, *41*, 7108–7146. [CrossRef]

4. Abbott, A.P.; Capper, G.; Davies, D.L.; McKenzie, K.J.; Obi, S.U. Solubility of Metal Oxides in Deep Eutectic Solvents Based on Choline Chloride. *J. Chem. Eng. Data* **2006**, *51*, 1280–1282. [CrossRef]

5. Hong, S.K.; Doughty, R.M.; Osterloh, F.E.; Zaikina, J.V. Deep eutectic solvent route synthesis of zinc and copper vanadate n-type semiconductors-mapping oxygen vacancies and their effect on photovoltage. *J. Mater. Chem. A* **2019**, *7*, 12303–12316. [CrossRef]

6. Hong, S.; Burkhow, S.J.; Doughty, R.M.; Cheng, Y.; Ryan, B.J.; Mantravadi, A.; Roling, L.T.; Panthani, M.G.; Osterloh, F.E.; Smith, E.A.; et al. Local Structural Disorder in Metavanadates MV₂O₆ (M = Zn and Cu) Synthesized by the Deep Eutectic Solvent Route: Photoactive Oxides with Oxygen Vacancies. *Chem. Mater.* **2021**, *33*, 1667–1682. [CrossRef]

7. Boston, R.; Foeller, P.Y.; Sinclair, D.C.; Reaney, I.M. Synthesis of Barium Titanate Using Deep Eutectic Solvents. *Inorg. Chem.* **2017**, *56*, 542–547. [CrossRef]

8. Thorat, G.M.; Jadhav, H.S.; Roy, A.; Chung, W.J.; Seo, J.G. Dual Role of Deep Eutectic Solvent as a Solvent and Template for the Synthesis of Octahedral Cobalt Vanadate for an Oxygen Evolution Reaction. *ACS Sustain. Chem. Eng.* **2018**, *6*, 16255–16266. [CrossRef]
9. Hong, S.; Cheng, Y.; Hariyani, S.; Li, J.Z.; Doughty, R.M.; Mantravadi, A.; Adeyemi, A.N.; Smith, E.A.; Brgoch, J.; Osterloh, F.E.; et al. The Deep Eutectic Solvent Precipitation Synthesis of Metastable Zn₄V₂O₉. *Inorg. Chem.* **2022**, *66*, 154–169. [CrossRef]

10. Zeng, J.R.; Chen, L.; Siwal, S.S.; Zhang, Q.B. Solvothermal sulfurization in a deep eutectic solvent; a novel route to synthesize Co-doped Ni₃S₂ nanosheets supported on Ni foam as active materials for ultrahigh-performance pseudocapacitors. *Sustain. Energy Fuels* **2019**, *3*, 1957–1965. [CrossRef]

11. Zhang, T.; Doert, T.; Ruck, M. Synthesis of Metal Sulfides from a Deep Eutectic Solvent Precursor (DESP). *Z. Anorg. Allg. Chem.* **2017**, *643*, 1913–1919. [CrossRef]

12. Jiang, J.Y.; Chang, L.Y.; Zhao, W.C.; Tian, Q.Y.; Xu, Q. An advanced FeCoNi nitro-sulfide hierarchical structure from deep eutectic solvents for enhanced oxygen evolution reaction. *Chem. Commun.* **2019**, *55*, 10174–10177. [CrossRef] [PubMed]

13. Hahn, H.; Frank, G.; Klinger, W.; Meyer, A.D.; Stöerger, G.; Anorg, Z. Untersuchungen über ternäre Chalkogenide. V. Über einige ternäre Chalkogenide mit Chalkopyritstruktur. *Z. Anorg. Allg. Chem.* **1953**, *271*, 153–170. [CrossRef]

14. Delgado, G.; Mora, A.J.; Pineda, C.; Tinoco, T. Simultaneous Rietveld refinement of three phases in the Ag-In-S semiconducting system from X-ray powder diffraction. *Mater. Res. Bull.* **2001**, *36*, 2507–2517. [CrossRef]

15. Roth, R.S.; Parker, H.S.; Brower, W.S. Comments on the system Ag₂S·In₂S₃. *Mater. Res. Bull.* **1973**, *8*, 333–338. [CrossRef]

16. Range, K.J.; Keubler, M.; Weiss, A. Eine Hochdruckmodifikation des AgInS₂ mit α-NaFeO₂-Structure. *Z. Naturforschg.* **1969**, *24*, 1060–1061. [CrossRef]

17. Shay, J.L.; Tell, B.; Schiavon, L.M.; Kasper, H.M.; Thiel, F. Energy bands of AgInS₂ in the chalcopyrite and orthorhombic structures. *Phys. Rev. B* **1974**, *9*, 1719–1723. [CrossRef]

18. Jain, A.; Shyue Ping, O.; Hautier, G.; Chen, W.; Richards, W.D.; Dacek, S.; Cholia, S.; Gunter, D.; Skinner, D.; Ceder, G.; et al. Commentary: The Materials Project: A materials genome approach to accelerating materials innovation. *APL Mater.* **2013**, *1*, 011002. [CrossRef]

19. Torimoto, T.; Adaichi, T.; Okazaki, K.-i.; Sakuraoka, M.; Shibayama, T.; Ohtani, B.; Kudo, A.; Kuwabata, S. Facile Synthesis of ZnS-AnInS₂ Solid Solution Nanoparticles for a Color-Adjustable Luminophore. *J. Am. Chem. Soc.* **2007**, *129*, 12388. [CrossRef]

20. Kowalik, P.; Penkala, M.; Bujak, P.; Kmita, A.; Gajewska, M.; Ostowski, A.; Slodek, A.; Pron, A. From Ag₂S to luminescent Ag-In-S nanocrystals via an ultrasonic method—In situ synthesis study in an NMR tube. *J. Mater. Chem. C* **2020**, *8*, 8942–8952. [CrossRef]

21. Chhikara, N.; Gupta, P.; Gupta, B.K.; Jain, K.; Chand, S. Synthesis of AgInS₂ nanoparticles Directly in Poly (3-hexyl thiophene) (P3HT) Matrix: Photoluminescence quenching studies. In *Physics of Semiconductor Devices*; Environmental Engineering; Springer: Cham, Switzerland, 2014; pp. 335–338.

22. Hamanaka, Y.; Ogawa, T.; Tsuzuski, M.; Kuzuya, T. Photoluminescence Properties and Its Origin of AgInS₂ Quantum Dots with Chalcopyrite Structure. *J. Phys. Chem. C* **2011**, *115*, 1786–1792. [CrossRef]

23. Uematsu, T.; Wajima, K.; Sharma, D.K.; Hirata, S.; Yamamoto, T.; Kameyama, T.; Vacha, M.; Torimoto, T.; Kuwabata, S. Narrow band-edge photoluminescence from AgInS₂ semiconductor nanoparticles by the formation of amorphous III-VI semiconductor shells. *NPG Asia Mater.* **2018**, *10*, 713–726. [CrossRef]

24. Park, Y.J.; Oh, J.H.; Han, N.H.; Yoon, H.C.; Park, S.M.; Do, Y.R.; Song, J.K. Phoyoluminescence of Band Gap States in AgInS₂ Nanoparticles. *J. Phys. Chem. C* **2014**, *118*, 25677–25683. [CrossRef]

25. Hong, S.P.; Park, H.K.; Oh, J.H.; Yang, H.; Do, Y.R. Comparisons of the structural and optical properties of o-AgInS₂, t-AgInS₂, and c-AgIn₅S₈ nanocrystals and their solid-solution nanocrystals with ZnS. *J. Mater. Chem.* **2012**, *22*, 18939–18949. [CrossRef]

26. Putz, H.; Brandenburg, K. Match!-Phase Analysis Using Powder Diffraction, Crystal Impact. Available online: https://www.crystalimpact.com/contact.htm (accessed on 20 December 2021).

27. *PDXL: Integrated X-ray Powder Diffraction Software*; Version 2.8.1.1; Rigaku: The Woodlands, TX, USA, 2018.

28. Chupas, P.J.; Chapman, K.W.; Kurtz, C.; Hanson, J.C.; Lee, P.L.; Grey, C.P. A versatile sample-environment cell for non-ambient X-ray scattering experiments. *J. Appl. Crystallogr.* **2008**, *41*, 822–824. [CrossRef]
9. Hong, S.; Cheng, Y.; Hariyani, S.; Li, J.Z.; Doughty, R.M.; Mantravadi, A.; Adeyemi, A.N.; Smith, E.A.; Brgoch, J.; Osterloh, F.E.; et al. The Deep Eutectic Solvent Precipitation Synthesis of Metastable Zn₄V₂O₉. *Inorg. Chem.* **2022**, *66*, 154–169. [CrossRef]

10. Zeng, J.R.; Chen, L.; Siwal, S.S.; Zhang, Q.B. Solvothermal sulfurization in a deep eutectic solvent; a novel route to synthesize Co-doped Ni₃S₂ nanosheets supported on Ni foam as active materials for ultrahigh-performance pseudocapacitors. *Sustain. Energy Fuels* **2019**, *3*, 1957–1965. [CrossRef]

11. Zhang, T.; Doert, T.; Ruck, M. Synthesis of Metal Sulfides from a Deep Eutectic Solvent Precursor (DESP). *Z. Anorg. Allg. Chem.* **2017**, *643*, 1913–1919. [CrossRef]

12. Jiang, J.Y.; Chang, L.Y.; Zhao, W.C.; Tian, Q.Y.; Xu, Q. An advanced FeCoNi nitro-sulfide hierarchical structure from deep eutectic solvents for enhanced oxygen evolution reaction. *Chem. Commun.* **2019**, *55*, 10174–10177. [CrossRef] [PubMed]

13. Hahn, H.; Frank, G.; Klinger, W.; Meyer, A.D.; Stöerger, G.; Anorg, Z. Untersuchungen über ternäre Chalkogenide. V. Über einige ternäre Chalkogenide mit Chalkopyritstruktur. *Z. Anorg. Allg. Chem.* **1953**, *271*, 153–170. [CrossRef]

14. Delgado, G.; Mora, A.J.; Pineda, C.; Tinoco, T. Simultaneous Rietveld refinement of three phases in the Ag-In-S semiconducting system from X-ray powder diffraction. *Mater. Res. Bull.* **2001**, *36*, 2507–2517. [CrossRef]

15. Roth, R.S.; Parker, H.S.; Brower, W.S. Comments on the system Ag₂S·In₂S₃. *Mater. Res. Bull.* **1973**, *8*, 333–338. [CrossRef]

16. Range, K.J.; Keubler, M.; Weiss, A. Eine Hochdruckmodifikation des AgInS₂ mit α-NaFeO₂-Structure. *Z. Naturforschg.* **1969**, *24*, 1060–1061. [CrossRef]

17. Shay, J.L.; Tell, B.; Schiavon, L.M.; Kasper, H.M.; Thiel, F. Energy bands of AgInS₂ in the chalcopyrite and orthorhombic structures. *Phys. Rev. B* **1974**, *9*, 1719–1723. [CrossRef]

18. Jain, A.; Shyue Ping, O.; Hautier, G.; Chen, W.; Richards, W.D.; Dacek, S.; Cholia, S.; Gunter, D.; Skinner, D.; Ceder, G.; et al. Commentary: The Materials Project: A materials genome approach to accelerating materials innovation. *APL Mater.* **2013**, *1*, 011002. [CrossRef]

19. Torimoto, T.; Adaichi, T.; Okazaki, K.-i.; Sakuraoka, M.; Shibayama, T.; Ohtani, B.; Kudo, A.; Kuwabata, S. Facile Synthesis of ZnS-AnInS₂ Solid Solution Nanoparticles for a Color-Adjustable Luminophore. *J. Am. Chem. Soc.* **2007**, *129*, 12388. [CrossRef]

20. Kowalik, P.; Penkala, M.; Bujak, P.; Kmita, A.; Gajewska, M.; Ostowski, A.; Slodek, A.; Pron, A. From Ag₂S to luminescent Ag-In-S nanocrystals via an ultrasonic method—In situ synthesis study in an NMR tube. *J. Mater. Chem. C* **2020**, *8*, 8942–8952. [CrossRef]

21. Chhikara, N.; Gupta, P.; Gupta, B.K.; Jain, K.; Chand, S. Synthesis of AgInS₂ nanoparticles Directly in Poly (3-hexyl thiophene) (P3HT) Matrix: Photoluminescence quenching studies. In *Physics of Semiconductor Devices*; Environmental Engineering; Springer: Cham, Switzerland, 2014; pp. 335–338.

22. Hamanaka, Y.; Ogawa, T.; Tsuzuski, M.; Kuzuya, T. Photoluminescence Properties and Its Origin of AgInS₂ Quantum Dots with Chalcopyrite Structure. *J. Phys. Chem. C* **2011**, *115*, 1786–1792. [CrossRef]

23. Uematsu, T.; Wajima, K.; Sharma, D.K.; Hirata, S.; Yamamoto, T.; Kameyama, T.; Vacha, M.; Torimoto, T.; Kuwabata, S. Narrow band-edge photoluminescence from AgInS₂ semiconductor nanoparticles by the formation of amorphous III-VI semiconductor shells. *NPG Asia Mater.* **2018**, *10*, 713–726. [CrossRef]

24. Park, Y.J.; Oh, J.H.; Han, N.H.; Yoon, H.C.; Park, S.M.; Do, Y.R.; Song, J.K. Phoyoluminescence of Band Gap States in AgInS₂ Nanoparticles. *J. Phys. Chem. C* **2014**, *118*, 25677–25683. [CrossRef]

25. Hong, S.P.; Park, H.K.; Oh, J.H.; Yang, H.; Do, Y.R. Comparisons of the structural and optical properties of o-AgInS₂, t-AgInS₂, and c-AgIn₅S₈ nanocrystals and their solid-solution nanocrystals with ZnS. *J. Mater. Chem.* **2012**, *22*, 18939–18949. [CrossRef]

26. Putz, H.; Brandenburg, K. Match!-Phase Analysis Using Powder Diffraction, Crystal Impact. Available online: https://www.crystalimpact.com/contact.htm (accessed on 20 December 2021).

27. *PDXL: Integrated X-ray Powder Diffraction Software*; Version 2.8.1.1; Rigaku: The Woodlands, TX, USA, 2018.

28. Chupas, P.J.; Chapman, K.W.; Kurtz, C.; Hanson, J.C.; Lee, P.L.; Grey, C.P. A versatile sample-environment cell for non-ambient X-ray scattering experiments. *J. Appl. Crystallogr.* **2008**, *41*, 822–824. [CrossRef]